Anal Bioanal Chem (2005) 383: 489–499 DOI 10.1007/s00216-005-0057-y
PA P E R I N F O R E F R O N T
Frank Ottinger . Ivana Kroslakova .
Kathrin Hametner . Eric Reusser . Reinhard Nesper . Detlef Günther
Analytical evidence of amorphous microdomains
within nitridosilicate and nitridoaluminosilicate
Received: 13 June 2005 / Accepted: 22 July 2005 / Published online: 15 September 2005
# Springer-Verlag 2005
Abstract Single crystals of new nitridosilicates and nitrido-aluminosilicates with excellent R values in X-ray inves-tigations were analysed quantitatively using 30 to 60 μm single-spot LA-ICP-MS. Significant discrepancies between expected and measured chemical composition could not be explained by the crystallographic data. High spatial reso-lution analysis using electron probe microanalysis (EPMA, 10 μm) leads to the discovery of inhomogeneities in the crystalline material. The application of standard single-spot LA-ICP-MS with a spatial resolution of 30 to 60μm is not suitable for the analysis of these crystals as the existing inhomogeneities dominate and alter the determined con-centrations. However, owing to the better detection capa-bilities, a scanning LA-ICP-MS procedure enables a more representative analysis of single crystals of Ca5Si2Al2N8
than single-spot LA-ICP-MS as a result of a larger sam-pling volume. It is highly likely that these impurities con-sist of amorphous, vitreous phases as powder diffraction X-ray data indicates the existence of a significant fraction of an X-ray amorphous material besides crystalline sili-cates. These microdomains contain less aluminium, silicon and calcium or are nearly free of aluminium, which explains the detected discrepancies in the chemical composition.
Keywords Nitridosilicates . Single crystals . Microprobe . LA-ICP-MS
Oxosilicates are the largest known class of minerals com-bining two of the most abundant elements in the earth’s crust. A very large number of oxosilicate phases with an enormous diversity of structures have been investigated, whereas nitrogen-containing silicates are relatively unex-plored [1–9]. Nitridosilicates can be derived from oxosil-icates by a formal exchange of oxygen with nitrogen, i.e. they contain SiN4instead of SiO4tetrahedra. Consequent-ly, the high possible degree of crosslinking in nitridosili-cates leads predominantly to three-dimensional network structures. The compounds exhibit outstanding chemical and physical stability and are of interest for this reason.
Among the wide variety of direct solid analysis tech-niques available, laser ablation inductively coupled plasma mass spectrometry (LA-ICP-MS) has become one of the major analytical methods to determine elemental concen-trations within solids [10–12]. The high sensitivity of this technique allows the direct determination of major, minor and trace elements within a spatial resolution of few tens of micrometres. Therefore, the major application of this technique is geology, where in situ trace element analysis within different mineral phases can be assessed . Fur-thermore, a variety of powder and sediment samples have been analysed to gain information about the trace element distribution, which can be used for studies into the climate and environmental pollution [14, 15]. However, recent studies in material science indicate a growing interest in applying this technique for trace element determinations in high-purity materials such as CaF2, the trace element
determination in zeolites  and furthermore measure-ments of element concentrations in Si-B-C-N high-durable ceramic materials . It has been shown that the detec-tion capabilities of the technique are sufficient to measure the trace element impurities in concentrations as low as few ng g−1. The major element concentration ratios were determined with a precision of approximately 2–5%. F. Ottinger . I. Kroslakova . K. Hametner .
R. Nesper . D. Günther (*)
ETH Zurich, Laboratory of Inorganic Chemistry, 8093 Zurich, Switzerland
e-mail: firstname.lastname@example.org E. Reusser
ETH Zurich, Institute for Mineralogy and Petrology, 8092 Zurich, Switzerland
Fundamental studies in LA-ICP-MS have shown that the sampling process, the aerosol transport and the excitation of the generated aerosols are still not fully understood , such that each new application requires a thorough vali-dation of the analytical data. Since the materials of interest within this study are synthetic samples and no external ref-erence materials for the quantification are available, a de-tailed analytical study on a variety of inorganic materials was carried out and the data were used to describe new synthesised nitridosilicates and nitridoaluminosilicates.
The aim of this study was to determine the stoichiomet-ric composition of nitridosilicates and possible
synthesis-derived impurities by using LA-ICP-MS. Since impurities are expected in the μg g−1 concentration range this tech-nique is most sensitive for multielement analysis of solids. Therefore, a variety of samples were analysed using spa-tially resolved analysis. The NIST 610 glass reference material was used for external calibration and Ca was used as internal standard. Since no matrix-matched calibration material was available for this study, mineral samples (Wollastonite and Grossular) with closely related composi-tion were also analysed. To verify the data acquired by LA-ICP-MS, electron probe microanalysis (EPMA) was also applied to selected samples for validation purposes. Fig. 1 Anionic network
struc-ture of Ca5Si2Al2N8. Closed
AlN4tetrahedra (dark green),
SiN4tetrahedra (yellow), Ca2+
cations (blue balls). View along 
Fig. 2 Anionic network struc-ture of Ca4SiAl3N7. Closed
AlN4tetrahedra (dark green),
mixed SiAlN4tetrahedra (light
green), SiN4tetrahedra (yellow),
Ca2+cations (blue balls). View along 
The synthesis and characterisation of nitridoaluminosili-cates or nitridosilinitridoaluminosili-cates with a low degree of condensation is challenging due to their reactivity and high affinity for hydrolysis or oxidation in air. In contrast, nitridosilicates with a high degree of condensation exhibit an extraordinary stability towards concentrated mineral acids or bases . We were able to open up a new synthetic pathway to the first nitridoaluminosilicates Ca5Si2Al2N8and Ca4SiAl3N7 as well as the nitridosilicate Ca7Si4N10 by reaction of binary calcium nitrides or subnitrides with silicon and/or aluminium in closed niobium or tantalum ampoules at
temperatures well above 1,200°C . These nitridoalu-minosilicates are the first structurally identified compounds of the last missing member in the AmTnXp family of silicates (A=cations; T=Si and/or Al; X=O and/or N).
All of the abovementioned new compounds exhibit a so far unknown structure type. Ca5Si2Al2N8and Ca4SiAl3N7 crystallise with three-dimensional network structures (Fig.1
and2) and can therefore be classified as tectosilicates, where-as Ca7Si4N10 with its puckered layered structure (Fig. 3) can be identified as a phyllosilicate. Although Ca5Si2Al2N8 and Ca4SiAl3N7possess a high degree of condensation (0.5 and 0.57), both compounds are not stable to diluted mineral acids in contrast to nitridosilicates with a similar degree of condensation. Not surprisingly, Ca7Si4N10decomposes when exposed to water due to its layered structure and its low degree of condensation.
The crystallographic investigation of single crystals of all three compounds leads to unambiguous structural solu-tions. They can all be refined down to very small R val-ues (Ca7Si4N10 2.65%, Ca5Si2Al2N8 1.61%, Ca4SiAl3N7 3.27%) leaving no space for structural speculations. We have found no crystallographic indication for mixed or not fully occupied atomic sites or for atoms heavier than Ca.
Since Si4+and Al3+or O2−and N3−have similar atomic form factors, a clear differentiation between these ions is very difficult and sometimes impossible based on X-ray data only. The allocation in Si4+ and Al3+ succeeds for Ca5Si2Al2N8 on the basis of Si–N and Al–N bond
distances, with Al–N bonds being significantly longer than Si–N bonds. Such a differentiation does not succeed for Ca4SiAl3N7 relying on X-ray diffraction experiments
only. The computation of Madelung factors, lattice ener-gies and point potentials permits the generation of a plausible Si/Al distribution for this compound .
Based on that data alone, one cannot exclude possible phase ranges for these compounds according to Ca7Si4−x
AlxN10−xOx, Ca5Si2−xAl2+xN8−xOxand Ca4Si1−xAl3+xN7−x
Ox, demonstrating their close relationship to sialons.
Fig. 3 Anionic layer structure of Ca7Si4N10. Closed SiN4
tet-rahedra (yellow), Ca2+cations (blue balls). View along 
Table 1 Operating conditions for laser sampling and ICP-MS measurements
Laser type ArF excimer
Laser wavelength 193 nm
Spot diameter (sample and standard) 30–60 μm Repetition rate sample 5 Hz Repetition rate standard 10 Hz
Laser energy 170 mJ
He carrier gas flow rate 1 L min−1
RF Power 1,410 W
Nebulizer gas flow rate 0.7 L min−1 Auxiliary gas flow rate 0.85 L min−1 Coolant gas flow rate 16 L min−1
Lens settings Autolens
Number of sweeps 2
Number of readings 320
Number of replicates 1
Dwell time 10 ms
Detector mode Dual (pulse and analog) Number of measured elements 11
Laser ablation sampling was performed using an ArF 193 nm excimer laser (GeoLas Q, MicroLas, Göttingen, Germany) which was coupled to an ICP-MS instrument (Elan 6100 DRC+Perkin Elmer, SCIEX, Concord, Ontario, Canada). The operating conditions of the instrumentation are summarised in Table1.
The samples were ablated in single crater mode at a spatial resolution of 60μm and a repetition rate of 5 and 10 Hz. Within an analysis sequence of 20 analyses, each individual analysis consisted of 30 s gas blank measure-ments followed by 60 s ablation of the sample. Standards were measured twice at the beginning of a run and twice at the end of the analyses. The quantification procedure was based on external calibration using NIST (National Institute for Standards and Technology), SRM 610 and in-ternal standardization. The use of an inin-ternal standard al-lows correction for differences in the mass ablated between the sample of interest and reference material, differences in the transport behaviour of the laser generated aerosols and also as drift correction for processes within the plasma . For analysis of solids in their natural state, a naturally oc-curring internal standard (e.g. calcium is very often the element of choice owing to its abundance in many miner-als) is recommended for quantification . The concen-tration of the element which is supposed to be used as internal standard must therefore be known prior to the analysis and should be homogeneously distributed within the sample of interest. We obtained the concentration of the internal standard element by calculating its concentration
from the stoichiometry of the mineral or using an alterna-tive method (in our case EPMA) to determine its concen-tration in the sample. Due to the atmospheric nature of the ICP, oxygen and nitrogen cannot be measured using this technique.
Calcium was chosen as an internal standard as a result of its crystallographic unambiguousness. Substitution of Al with Si and N with O for Ca5Si2Al2N8 could lead to a
possible phase width Ca5Si2−xAl2+xOxN8−x with 0≤x≤2.
The analyses revealed that this range shows an upper lim-it of x=0.6. Nevertheless, calcium is the most sulim-itable internal standard owing to the negligible change in overall mass shown in Table2. Even at x=0.6 the mass fraction of Ca declines marginally from 47.42 wt% to 47.36 wt%. The implemented uncertainty by the standardization is sig-nificantly below the precision of the method and can therefore be neglected for this investigated phase. The same argumentation is valid for Ca7Si4−xAlxN10−xOxand
Before analysing the synthetic samples, the quantifica-tion procedure was tested using minerals. To investigate the ablation behaviour of Ca in relation to Al and Si, Grossular and Wollastonite minerals with closely matched composi-tions were analyzed within this study. These studies were of importance since matrix effects in the ICP may occur, which are also called “elemental fractionation effects” [23–26].
Quantification of Grossular was based on Ca as internal standard. The Ca concentration was calculated from the Table 2 Variation of the mass
distribution in Ca5Si2−xAl2+x OxN8−xwith 0≤x≤0.6 x Formula M (g mol−1) wt% Ca Si Al O N 0 Ca5Si2Al2N8 422.58 47.42 13.30 12.77 0 26.52 0.1 Ca5Si1.9Al2.1O0.1N7.9 422.67 47.41 12.63 13.41 0.38 26.18 0.2 Ca5Si1.8Al2.2O0.2N7.8 422.76 47.40 11.96 14.04 0.76 25.84 0.3 Ca5Si1.7Al2.3O0.3N7.7 422.84 47.39 11.29 14.68 1.14 25.51 0.4 Ca5Si1.6Al2.4O0.4N7.6 422.93 47.38 10.63 15.31 1.51 25.17 0.5 Ca5Si1.5Al2.5O0.5N7.5 423.02 47.37 9.96 15.95 1.89 24.83 0.6 Ca5Si1.4Al2.6O0.6N7.4 423.11 47.36 9.20 16.58 2.27 24.50
Table 3 Results of LA-ICP-MS analysis of Grossular using Ca as internal standard
Ca concentration applied for quantification was based on stoichiometry and concentra-tions determined by EPMA
Measurement Measured concentrations (wt%)
42Ca: Theoretical 42Ca: EPMA 27 Al 29Si 42Ca 27Al 29Si 42Ca 1 8.77 19.57 26.69 8.66 19.33 26.76 2 8.95 19.15 26.69 8.85 18.92 26.76 3 8.96 19.24 26.69 8.85 19.01 26.76 4 8.68 19.54 26.69 8.58 19.30 26.76 5 8.61 19.38 26.69 8.51 19.15 26.76 Summary Average (wt%) 8.8 19.4 26.7 8.7 19.1 26.8 Standard deviation (wt%) 0.16 0.18 – 0.16 0.18 – RSD (%) 1.79 0.95 – 1.84 0.93 – Recovery (%) 73.4 103.7 – 86.1 105.3 –
stoichiometry (Ca=26.69 wt%) and the concentration deter-mined by EPMA measurement (Ca=26.37 wt%, see Table3). The theoretical composition of Grossular, Ca3Al2Si3O12,
was calculated from its stoichiometry: Ca=26.69 wt%, Al=11.98 wt%, Si=18.70 wt%. The experimental element distribution of that mineral determined from EPMA mea-surements shows a different composition: Ca=26.76±0.08 wt%, Al=10.25±0.26 wt%, Si=18.45±0.15 wt%.
For further evaluation of the accuracy of the Ca/Si concentration ratios, another naturally occurring mineral Wollastonite (CaSiO3) was analysed. The theoretical
com-position of Wollastonite was calculated from its stoichi-ometry: Ca=34.50 wt%, Si=24.18 wt%. Three Wollastonite minerals, Quebec, Bazene and Oravitza, obtained from different regions were analysed with the corresponding concentration ratios summarized in Table4. The recovery of the Si concentration based on internal standardization using Ca within natural minerals indicates the suitability of LA-ICP-MS for these types of samples. Therefore, it can be concluded that the analysis of nitrogen-containing silicate samples using the same analytical procedure should lead to similar results.
The electron probe microanalysis (EPMA) was per-formed on a JEOL JXA 8200 instrument equipped with a 5-wavelength dispersive X-ray spectrometer (WDS) and an energy dispersive spectrometer (EDS). Electron beam
con-ditions for quantitative analysis and image acquisition were an acceleration voltage of 15 kV, a beam current of 15 nA and a beam diameter <100 nm. The X-ray lines selected for analysis were Ca K at a wavelength of 0.33595 nm, Al K at 0.83401 nm and Si K at 0.71262 nm. The monochromator crystals used were PET for Ca and TAP for Al and Si.
The standards used were pure CaCO3 (calcite) crystals
for calcium, pure Al2O3 (corundum) for aluminium and
pure SiO2(quartz) for silicon. The sample was coated with
a 20-nm layer of carbon. All measurements were corrected for detector dead time, instrumental drift and X-ray back-ground. For the correction of the inter-element effects (i.e. absorption, fluorescence) the CITZAF code was applied . Nitrogen was not measured directly because of the strong absorption of its X-ray radiation by the matrix lead-ing to big uncertainties. Therefore, nitrogen was calculated by difference to 100%.
Results and discussion
Since the early application of laser ablation, Ca has always been the preferred internal standard for trace element de-terminations . However, ablation studies using a 266-nm laser ablation system revealed that Ca/Si ratios can vary significantly . More recent investigations on the influ-ence of the wavelength on the ablation behaviour of var-ious matrices have shown that the shorter wavelength leads to significantly reduced fractionation effects [28–30]. Fur-thermore, recent studies on the stoichiometric composition of laser-generated aerosols also indicated that the stoichio-metric composition of the material entering the excitation source represents the original sample . Therefore it can be concluded that any deviation of the ICP-MS signal in-tensities measured must be influenced by different ioniza-tion of particles of the reference material (NIST 610) and the sample within the ICP. However, since it is also known that 193 nm produces the smallest particle fractions (ca. below 200 nm), these effects should be significantly re-duced . The results on natural minerals summarised in Table 3 acquired using 193 nm demonstrate that the achievable precision and accuracy for these types of samples and deviations as obtained in ref.  were not observed. Therefore, LA-ICP-MS analyses on a single Table 4 Results of the LA-ICP-MS analysis of Wollastonite
min-erals using Ca (34.50 wt% based on theoretical values) as internal standard
Measurement Measured concentrations (wt%) Quebec Bazene Oravitza 42 Ca 29Si 29Si 29Si 1 34.50 25.01 23.75 23.42 2 34.50 24.07 24.54 24.12 3 34.50 24.17 24.12 22.76 4 34.50 24.31 24.31 23.23 5 34.50 24.07 24.12 23.18 Summary Average (wt%) 34.5 24.3 24.2 23.3 Standard deviation (wt%) – 0.39 0.29 0.50 RSD (%) – 1.60 1.20 2.14 Recovery (%) – 100.6 100.0 96.5
Table 5 Results of the LA-ICP-MS analyses of a single crystal of Ca5Si2Al2N8using Ca (47.42 wt% based on theoretical values) as internal and NIST 610 as external standard, all concentrations inμg g−1
Isotope 7Li 23Na 25Mg 27Al 28Si 29Si 30Si 35Cl 42Ca 43Ca 44Ca 57Fe 88Sr 93Nb 153Eu Replicate 1 46 88 10 136,800 96,800 98,000 99,100 29 474,200 456,100 403,900 123 45 101 1 Replicate 2 26 106 7 133,400 98,600 98,400 98,900 57 474,200 461,300 459,300 135 46 85 1 Replicate 3 115 506 10 134,800 95,000 93,600 93,000 47 474,200 452,100 413,200 113 41 47 1 Replicate 4 4 1 8 137,900 100,700 99,600 100,600 45 474,200 491,000 470,000 100 44 44 1 Replicate 5 14 36 7 134,300 103,800 102,200 99,500 50 474,200 461,100 468,100 123 45 91 1 Average 41 147 8 135,400 99,000 98,400 98,300 46 474,200 464,300 442,900 119 44 74 1 Standard deviation 44 204 1 1,800 3,400 3,100 2,900 10 15,400 31,800 14 2 26 0
crystal of Ca5Si2Al2N8were carried out to investigate the Al/Si concentration ratio as well as the concentration and distribution of trace element impurities. The concentrations of the single-spot analyses are summarised in Table5.
Five replicate single-spot analyses were carried out on the same single crystal. Quantification was based on NIST 610 and internal standardization using Ca (42Ca using the nominal concentration of 47.42 wt% in Ca5Si2Al2N8). The
isotopes 7Li, 11B, 23Na, 25,26Mg, 27Al, 28,29,30Si, 35,37Cl,
153Eu,178Hf and181Ta with limits of detection of 1–10 ng g−1
were measured. Only the elements given in the table were significantly above the limits of detection. The ubiquitous occurrence of sodium was detected at an average concen-tration of 147μg g−1. However, the precision indicates a highly variable distribution of this element within the synthesized crystal. Li, Mg, Cl, Fe, Sr, Nb and Eu are trace elements present in the single crystal with a maximum concentration of 100μg g−1(1–119 μg g−1). These results indicate that this single crystal consists mainly of calcium, silicon and aluminium without further significant impu-rities (Table6).
However, the determined concentrations of Al and Si were determined to be significantly different from their theoretical concentration. The sum of both elements was theoretically expected to be 26.06 wt% instead of the detected 23.43 wt%. The absolute difference of 2.63 wt% from the expected value or the relative deviation of 11.2% was also not explainable by a contribution of other ele-ments present in the matrix. The individual concentration of Al at 13.54±0.18 wt% was significantly higher than its expected value of 12.77 wt%. In contrast, the concentration of Si at 9.89±0.34 wt% was determined to be significantly below the theoretical value of 13.29 wt%.
To elucidate the influence of interferences, three dif-ferent isotopes were measured for Ca and Si. Excluding the contribution of mass bias, no significant influences due to interferences were obtained. Therefore, possible contribu-tions of14N14N14N,28Si14N,29Si14N or28Si16O clusters on the isotopes 42Ca, 43Ca or 44Ca can be excluded to be responsible for the underestimation of Si and slight over-estimation of Al. However, in the case of an interference on the internal standard, both elements would be influenced in Table 7 Results of the LA-ICP-MS analyses of a single crystal of Ca7Si4N10using Ca (52.64 wt% based on theoretical values) as internal and NIST 610 as external standard, all concentrations inμg g−1
Isotope 7Li 23Na 25Mg 27Al 29Si 30Si 35Cl 42Ca 43Ca 44Ca 57Fe 88Sr 93Nb Replicate 1 1 1 134 31,500 136,300 129,800 236 526,400 494,200 482,200 25 109 125 Replicate 2 1 1 165 26,200 162,000 15,020 220 526,400 514,300 490,500 24 110 284 Replicate 3 5 2 162 20,900 137,200 130,000 206 526,400 488,500 487,400 53 107 265 Replicate 4 1 1 147 29,200 151,600 145,000 335 526,400 527,700 484,300 14 123 245 Replicate 5 1 1 151 23,700 150,300 142,300 188 526,400 517,500 491,400 21 118 261 Average 2 1 152 26,300 147,500 139,500 237 526,400 508,400 487,100 27 113 236 Standard deviation 2 1 13 4,200 10,800 9,100 58 16,400 3,900 15 7 64
Table 8 Results of the LA-ICP-MS analyses of twelve single crystals of Ca5Si2Al2N8using NIST 610 and BCR 2G as an external standard and calcium as an internal standard
Al Si Σ Al+Si Absolute difference Crystal 1 13.54 9.89 23.43 2.63 Crystal 2 11.58 10.73 22.31 3.75 Crystal 3 11.16 10.00 21.16 4.90 Crystal 4 12.08 9.65 21.73 4.33 Crystal 5 12.29 10.85 23.14 2.92 Crystal 6 12.34 10.72 23.06 3.00 Crystal 7 11.59 10.24 21.83 4.23 Crystal 8 12.14 10.30 22.44 3.62 Crystal 9 12.05 10.57 22.62 3.44 Crystal 10 12.61 10.60 23.21 2.85 Crystal 11 10.82 10.51 21.33 4.73 Crystal 12 11.48 9.66 21.14 4.92 Average 11.97 10.31 22.28 3.78 Standard deviation 0.72 0.42 1.14 1.14
All concentrations are given in wt%. The last column shows the absolute difference to the expected sum value of 26.06 wt%
Table 6 Results of the LA-ICP-MS analyses of a single crystal of Ca4SiAl3N7using Ca (43.63 wt% based on theoretical values) as internal and NIST 610 as external standard, all concentrations inμg g−1
Isotope 7Li 23Na27Al 28Si 29Si 30Si 35Cl 42Ca 43Ca 44Ca 57Fe 88Sr 90Zr 93Nb 153Eu 181Ta Replicate 1 1 2 231,400 48,100 42,000 39,900 42 436,300 429,600 377,900 100 25 1 11,000 1 8 Replicate 2 36 1 231,700 46,600 45,200 42,500 43 436,300 449,100 437,800 97 24 1 11,400 1 7 Replicate 3 4 27 220,400 41,900 39,000 37,700 51 436,300 417,100 374,300 103 24 2 22,700 1 17 Replicate 4 3 2 214,400 43,700 39,100 38,700 52 436,300 421,500 372,700 105 25 1 23,100 1 17 Replicate 5 59 13 212,300 47,000 44,500 42,900 50 436,300 423,100 375,900 104 24 1 11,700 1 9 Average 21 9 222,000 45,400 42,000 40,400 48 436,300 428,092 387,700 102 24 1 13,000 1 12 Standard deviation 26 11 9,200 2,600 2,900 2,300 5 12,600 28,000 3 1 0 6,300 0 5
the same direction. EDX analyses also show the exclusive presence of Ca, Si, Al and N/O. Furthermore, we have no evidence for the presence of carbon as all displacement parameters are in the typical range for nitridosilicates or nitridoaluminates. Hydrogen can be excluded as a result of the reaction conditions as niobium or tantalum gets trans-parent to hydrogen at temperatures above 600°C .
Ca4SiAl3N7 is closely related to Ca5Si2Al2N8and was
therefore also investigated with the LA-ICP-MS method as there are no standards known for the Ca/Si/Al/N system. The results of the LA-ICP-MS analyses are summarised in Table4.
Five replicate single-spot analyses were carried out on the same single crystal. Quantification was based on NIST 610 and internal standardisation using Ca (42Ca using the nominal concentration of 43.63 wt% in Ca4SiAl3N7). The
isotopes 7Li,11B, 23Na, 25Mg,27Al, 28,29,30Si,35Cl, 39K,
Cr, 55Mn, 54,56,57Fe, 72Ge, 88Sr, 90Zr, 93Nb,
Eu,178Hf and181Ta with limits of detection in the order of 1–10 ng g−1were measured. Only the elements given in the table were significantly above the limits of detec-tion. The ubiquitous occurrence of sodium was detected at an average concentration of 9 μg g−1. Li, Cl, Fe, Sr, Zr, Eu and Ta and Eu are trace elements present in the single crystal with a maximum concentration of 100μg g−1 (1–102 μg g−1).
This crystal had a niobium concentration of 1.3 wt%, which can be interpreted by an inclusion of niobium in the single crystal, since the synthesis was performed in a closed niobium ampoule. We have no crystallographic evidence that Nb3+ is included in the crystal structure of Ca4SiAl3N7based on a detailed analysis of the structural
data. Looking at the time-dependent ablation signal of
93Nb, there is a maximum of the signal at the beginning and
at the end of the measurement, pointing to metallic niobium located at the surface of the crystal. Another spike in the signal points to a metallic inclusion in the crystal. The Fig. 4 Electron microscope picture using secondary electrons of
single crystals of Ca5Si2Al2N8embedded in methacrylate resin
Fig. 5 Electron microscope picture using back-scattered electrons of single crystals of Ca5Si2Al2N8embedded in methacrylate resin
Fig. 6 Threefold zoom of the framed area from Fig.5. Cap-tions highlight the different areas in the single crystal
corresponding signal increases by a factor of 50 in these areas.
However, the determined concentrations of Al and Si were determined to be significantly different from their theoretical concentration similar to Ca5Si2Al2N8. The sum of both elements was theoretically expected to be 29.68 wt % instead of the detected sum of 26.75 wt%. The absolute difference of 2.93 wt% from the expected value or the relative deviation of 9.9% was also not explainable by a contribution of another element present in the matrix. The individual concentration of Al at 22.21±0.91 wt% is very close to its expected concentration of 22.02 wt%. In contrast, the concentration of Si at 4.54±0.26 wt% was determined to be significantly below the theoretical value of 7.65 wt%.
Moreover, the quantitative analysis of a second crystal of Ca4SiAl3N7 leads to concentrations of Al and Si below
expectations once again. The concentration for Al and Si are at 20.08±1.99 wt% and 4.50±0.31 wt%, respectively. The absolute discrepancy between expected and measured concentration is at 5.10 wt% with aluminium having a very high standard deviation pointing to a less homogeneous distribution of aluminium throughout the crystal.
Identical investigations were also performed on single crystals of Ca7Si4N10 as there is no standard known for
the Ca/Si/N system. All determined concentrations were
standardized on 42Ca using the nominal concentration of 52.64 wt% in Ca7Si4N10. The concentrations of the LA-ICP-MS analyses on a Ca7Si4N10single crystal are sum-marised in Table7.
39K, 42–44Ca, 57Fe, 88Sr, 93Nb und 153Eu with limits of
detection in the order of 1–10 ng g−1were measured. Only the elements given in the table were significantly above the limits of detection. The ubiquitous occurrence of sodium was not detected in this single crystal. Li, Mg, Cl, Fe, Sr and Nb are trace elements present in the single crystal with a maximum fraction of 237 ppm (1–237 μg g−1).
Sur-prisingly, this single crystal contains 2.63 wt% of alumin-ium pointing to a composition of Ca7Si4−xAlxN10−xOxwith
Nevertheless, the concentrations for Al and Si of 17.38 wt% were determined to be significantly different from their expected theoretical concentration. The sum concen-tration of both elements was expected to be 21.06 wt% instead of the detected 17.38 wt%. The absolute difference of 3.68 wt% from the expected value or the relative de-viation of 21.1% was also not explainable by a contribu-tion of other elements present in the matrix. The silicon concentration of 14.75±1.08 wt% points to significant dif-ferences in concentration throughout the crystal due to its high standard deviation.
The sum of the Al and Si concentrations in the first analysed Ca5Si2Al2N8single crystal was the largest (23.43
wt%) measured out of twelve different single crystals of Ca5Si2Al2N8. The compositions and crystallographic
prop-erties of all these single crystals were thoroughly inves-tigated by X-ray diffraction before subsequent single-spot LA-ICP-MS analyses. Table 8summarises the Al and Si concentrations determined within these twelve crystals using two different external standards (NIST 610 and BCR2G). Both external reference materials (different in Table 9 Elemental analysis of the homogeneous grey area shown
in Fig.6using EPMA
Ca Al Si Σ Al+Si Absolute difference Spot 1 44.80 13.17 10.46 23.63 2.43 Spot 2 44.79 12.88 10.63 23.51 2.55 Spot 3 45.24 13.48 10.18 23.66 2.40 Spot 4 45.49 13.44 10.67 24.11 1.95 Spot 5 43.77 12.83 10.50 23.33 2.73 Spot 6 45.73 13.60 10.57 24.17 1.89 Average 44.97 13.23 10.50 23.74 2.32 Norm 47.42 13.95 11.07 25.02 1.04 Standard deviation 0.73 0.34 0.19 0.53 0.53 All concentrations in wt%. Denoted are the concentrations for Ca, Al and Si, their sum and the absolute difference to the expected value of 26.06 wt%
Table 10 Elemental analysis of the bright (spots 7 and 8) and dark areas (spots 9–11) shown in Fig.6using EPMA
Ca Al Si Spot 7 52.32 0.09 35.74 Spot 8 52.52 0.11 34.03 Spot 9 37.92 5.84 6.12 Spot 10 38.54 6.29 5.88 Spot 11 42.68 7.19 5.89
Concentrations for Ca, Al and Si are in wt%
Fig. 7 Electron microscope picture using back-scattered electrons of single crystals of Ca5Si2Al2N8embedded in methacrylate resin.
Areas investigated by scanning (3, 4, 7–9) or single-spot (b3–b8) LA-ICP-MS are marked with white lines or circles
their absorptivity) were used to exclude matrix effects within the ICP. The concentrations determined using both reference materials are insignificantly different.
The average concentrations were 11.97±0.72 wt% for Al and 10.31±0.42 wt% for Si. The overall deviation of the determined concentration and the theoretical sum concen-tration Al+Si is at 3.78 wt%. Considering a total standard deviation of 1.14 wt%, the difference to the theoretical concentration remains significant. Furthermore, the multi-element analysis results indicate that no other major ele-ment was impleele-mented into the crystal during synthesis.
Based on the concentration determination of Si and Al within Ca7Si4N10, Ca4SiAl3N7 and Ca5Si2Al2N8 and the results obtained on natural minerals it was necessary to use another analytical technique for cross validation of the results. Due to the fact the major element concentration differs by few wt%, EPMA at higher spatial resolution (10 instead of 60 μm), element-specific calibration and high suitability for major elements were applied to the same samples to get further insight into the Si/Al concentration ratios.
Therefore, single crystals of Ca5Si2Al2N8 were em-bedded in a methacrylate resin, the surface was polished and coated with a 20-nm layer of carbon. A thorough ex-amination of the polished single crystals reveals red in-clusions in the otherwise yellow crystals. One of these crystals and some of its splinters are shown in Fig.4. The pictures were taken using an electron microscope with secondary electrons. The crystalline material appears light grey, the methacrylate resin dark grey. The surface
rough-ness of some micrometers has no influence for the deter-mination of the composition.
Figure5shows the same area as in Fig.4but using back-scattered electrons. Different compositions result in differ-ent shades between light and dark grey. The outlined area in Fig.5shows several regions of different density and was therefore magnified three times as displayed in Fig.6.
Three different, analytically relevant regions were iden-tified (see Fig.6): a homogeneous medium grey region, an aluminium-free light grey region and a dark grey Ca-, Si-and Al-poor region. Marginal cavities filled with crystal debris were not investigated and appear in a very light grey. Table9shows the results of the elemental analysis of the homogeneous grey area shown in Fig.6using EPMA. As there are no internal but external standards only for this investigation, the detected value for calcium was normal-ised to the nominal concentration of 47.42 wt% (cf. line “norm”).
The EPMA analyses shows that the aluminium value is 2.0 wt% higher than the average concentration determined by LA-ICP-MS (Table 8), whereas the silicon concentra-tion increases by 0.8 wt%. That results in a sum concen-tration of Al+Si of 25.02±0.53 wt%, which is significantly higher in comparison to the 22.28 wt% determined by LA-ICP-MS (Table 8). The concentrations of aluminium, calcium and silicon are reproducible throughout the entire homogeneous area of the crystal. This value is in good agreement with the theoretical sum concentration of 26.06 wt% when considering the standard deviation of 0.53 wt%. Based on the analysis of the homogeneous area one Table 11 Results of the scanning mode LA-ICP-MS analysis of Ca5Si2Al2N8measured along the lines 3, 4, 7–9
7 Li 11B 25Mg 27Al 29Si 30Si 42Ca 43Ca 44Ca 57Fe 88Sr 93Nb Replicate“3” 0 1 32 134,300 113,300 105,400 474,200 477,900 471,500 484 48 269 Replicate“4” 5 1 90 137,600 114,800 107,200 474,200 475,200 471,700 499 51 223 Replicate“7” 1 1 39 139,800 116,500 111,300 474,200 475,500 469,800 471 47 135 Replicate“8” 0 2 33 147,200 99,900 97,700 474,200 474,000 466,700 451 51 202 Replicate“9” 1 1 18 143,200 117,300 111,800 474,200 474,300 475,600 444 46 154 Average 1 1 42 140,420 112,360 106,680 474,200 475,380 471,060 470 49 197 Standard deviation 2 0 28 5,000 7,100 5,700 1,500 3,200 23 3 54
Ca was used as an internal standard, NIST 610 as an external standard, all concentrations inμg g−1. The concentrations represent average concentrations of the analysed area
Table 12 Results of the 30-μm single-spot LA-ICP-MS analyses of the embedded Ca5Si2Al2N8single crystal using calcium as an internal standard, NIST 610 as an external standard; all concentrations inμg g−1
Isotope 7Li 11B 25Mg 27Al 29Si 30Si 42Ca 43Ca 44Ca 57Fe 88Sr 93Nb Replicate“b3” 0 1 12 128,300 109,500 104,400 474,200 481,500 476,800 432 52 254 Replicate“b4” 0 1 8 131,900 109,000 107,300 474,200 530,500 480,400 460 47 282 Replicate“b5” 0 1 2 131,000 106,100 108,400 474,200 475,700 477,900 424 43 139 Replicate“b6” 0 1 11 127,000 108,400 102,500 474,200 463,500 462,800 455 56 130 Replicate“b7” 0 1 6 133,200 106,000 106,000 474,200 475,000 476,000 448 66 223 Replicate“b8” 1 2 8 123,600 113,200 106,700 474,200 485,200 472,700 428 89 99 Average 0 1 8 129,167 108,700 108,700 474,200 485,233 474,433 441 59 188 Standard deviation 0 0 3 3,600 2,700 2,100 23,400 6,200 5 17 75
can derive an empirical formula of Ca5Si1.7 Al2.2OxN8−x
(x≅0.25) where values for oxygen and nitrogen were es-timated based on the electroneutrality. Two other single crystals of this material were analysed in a similar manner revealing the following compositions: Ca5Si1.7Al2.2OxN8−x
(x≅0.25) and Ca5Si1.5Al2.4OxN8−x(x≅0.45).
However, the EPMA analysis of the other light (spots 7+8) and dark grey areas (spots 9–11) lead to concentra-tions, which indicate different phase composition within the same single crystal. Table 10 summarises the results of these areas.
The light grey areas are nearly free of aluminium with a Ca:Si mass ratio of 1.5:1, whereas the dark grey areas contain less aluminium, silicon and calcium compared to the homogeneous region. These dark areas appear red and transparent when examined through an optical microscope and cannot be assigned to any known nitridoaluminosili-cate. Silicides and aluminidesilicides can be excluded due to the transparent appearance of the entire material and the missing difference to 100 wt%. Therefore, we can only conclude that these regions could consist of unknown crystalline silicates or amorphous, vitreous materials. How-ever, the exact determination has been unsuccessful so far. For a verification of the results of the EPMA analysis, LA-ICP-MS was used in scanning mode, in which the laser samples a larger area across the crystal. The purpose of this study was to explain the different concentrations deter-mined by single-spot LA-ICP-MS and EPMA analysis. Scanning mode LA-ICP-MS allows a continuous monitor-ing of the elemental composition of different sample areas. The sample is therefore moved during the laser sampling process. A similar type of 193 nm ArF excimer laser (Geolas Q, MicroLas Göttingen) with a spatial resolution of 30 μm was used for sample ablation. The well-char-acterized sample (Fig. 7) was used again for the scanning laser analyses. The 20-nm carbon coating on the surface was removed to prevent the formation of 12C16O and a subsequent interference on 28Si. The scanning mode was performed along the lines (3–9) shown in Fig. 7. Further-more, a comparison with the single-spot method using a 30-μm-diameter laser was also carried out (b3–b8). The results of the scanning mode LA-ICP-MS are summarised in Table11.
The sum concentration of Al+Si for the scanned areas led to an average concentration of 25.28±1.31 wt%, which is in good agreement with the theoretical and expected concentration of 26.06 wt%. The lower concentrations for
27Al in scan “3” and “4” are possibly caused by Al-free
regions as demonstrated by EPMA. These results show that the resultant concentrations describe the sample in a more lifelike way than the single-spot method.
An additional investigation of the abovementioned crystal with a 30-μm single-spot LA-ICP-MS leads not surprisingly to sum concentrations of Al and Si which are too low due to the detected inhomogeneities in the crystal. Table12gives the results of this investigation.
The chemical composition of single crystals investigated by X-ray was analyzed quantitatively using single-spot LA-ICP-MS. The cooperative use of a microprobe and a raster LA-ICP-MS leads to the discovery of inclusions in single crystals of Ca5Si2Al2N8. These impurities were not
detected by standard X-ray examination methods. It is likely that these impurities consist of either cocrystallised oxo- or nitridosilicates or amorphous, vitreous phases. X-ray powder diffraction data indicates the existence of a significant fraction of an X-ray amorphous material besides crystalline silicates. The application of a standard single-spot LA-ICP-MS with a spatial resolution of 60 or 30μm is not suitable for the analysis of these crystals as the existing inhomogeneities dominate and alter the determined con-centrations. This single-spot method always yields concen-trations for the sum of Al and Si for these crystals which are too low in comparison to the theoretical values. High spatial resolution analysis using EPMA (10 μm) leads to the discovery of inhomogeneities in the crystalline ma-terial. However, owing to the better detection capabilities, a scanning LA-ICP-MS procedure enables a more rep-resentative analysis of single crystals of Ca5Si2Al2N8than
single-spot LA-ICP-MS as a result of a larger sampling volume.
The excellent R factors of the single crystals derived from X-ray analysis of between 1.5 and 3.0 give no in-dication for these differences in composition. Therefore, we assume that these crystals are intergrown with unknown crystalline, amorphous or vitreous phases related to oxo- or nitridosilicates.
Acknowledgements This work was supported by ETH Zurich and the Swiss National Science Foundation.
1. Lissner F, Schleid T (2004) Z Anorg Allg Chem 630:2226– 2230
2. Gál ZA, Mallinson PM, Orchard HJ, Clarke SJ (2004) Inorg Chem 43:3998–4006
3. Orth M, Schnick W (1999) Z Anorg Allg Chem 625:1426– 1428
4. Huppertz H, Schnick W (1998) Z Anorg Allg Chem 624:371– 374
5. Huppertz H, Schnick W (1997) Z Anorg Allg Chem 623:212– 217
6. Huppertz H, Schnick W (1997) Angew Chem 109:2765–2767; Angew Chem Int Ed Engl 36:2651–2652
7. Huppertz H, Schnick W (1997) Acta Crystallogr Sect C53: 1751–1753
8. Huppertz H, Schnick W (1997) Chem Eur J 3:249–252 9. Huppertz H, Schnick W (1997) Chem Eur J 3:679–683 (For an
overview of publications on nitridosilicates published before 1997)
10. Durrant SF (1999) J Anal At Spectrom 14:1385–1404 11. Günther D, Jackson SE, Longerich HP (1999) Spectrochim
12. Becker JS, Pickhardt C, Dietze HJ (2000) Mikrochim Acta 135:71–80
13. Heinrich CA, Pettke T, Halter WE, Aigner-Torres M, Audetat A, Günther D, Hattendorf B, Bleiner D, Guillong M, Horn I (2003) Geochim Cosmochim Acta 67:3473–3497
14. Sinclair DJ, Kinsley LPJ, Mcculloch MT (1998) Geochim Cosmochim Acta 62:1889–1901
15. Baker SA, Bi M, Aucelio RQ, Smith BW, Winefordner JD (1999) J Anal At Spectrom 14:19–26
16. Koch J, Feldmann I, Hattendorf B, Günther D, Engel U, Jakubowski N, Bolshov M, Niemax K, Hergenroder R (2002) Spectrochim Acta B57:1057–1070
17. Pickhardt C, Brenner IB, Becker JS, Dietze HJ (2000) Fresenius J Anal Chem 368:79–87
18. Haberecht J, Hametner K, Nesper R, Günther D (2005) Chem Mat (in press)
19. Russo RE, Mao XL, Liu HC, Gonzalez J, Mao SS (2002) Talanta 57:425–451
20. Ottinger F (2004) Dissertation No. 15624, ETH Zurich, Switzerland
21. Longerich HP, Jackson SE, Günther D (1996) J Anal At Spectrom 11:899–904
22. Jackson SE, Longerich HP, Dunning GR, Freyer BJ (1992) Can Mineral 30:1049–1064
23. Fryer BJ, Jackson SE, Longerich HP (1995) Can Mineral 33:303–312
24. Longerich HP, Günther D, Jackson SE (1996) Fresenius J Anal Chem 355:538–542
25. Kuhn HR, Guillong M, Günther D (2004) Anal Bioanal Chem 378:1069–1074
26. Guillong M, Kuhn HR, Günther D (2003) Spectrochim Acta B58:211–220
27. Armstrong JT (1993) In: Proceedings of the 27th Annual MAS Meeting. Caltech, pp S13–14
28. Jeffries TE, Jackson SE, Longerich HP (1998) J Anal At Spectrom 13:935–941
29. Jeffries TE, Perkins WT, Pearce NJG (1995) Analyst 120: 1365–1372
30. Guillong M, Horn I, Günther D (2003) J Anal At Spectrom 18:1224–1230
31. Kuhn HR, Günther D (2004) J Anal At Spectrom 19:1158– 1164
32. Leon-Escamilla EA, Corbett JD (1998) J Alloys Compd 265: 104–114